Compressive strength

Compressive strength or compression strength is the capacity of a material or structure to withstand loads tending to reduce size, as opposed to Tensile strength which withstands loads tending to elongate. In other words, compressive strength resists being pushed together, whereas tensile strength resists tension (being pulled apart). In the study of strength of materials, tensile strength, compressive strength, and shear strength can be analyzed independently.
Some materials fracture at their compressive strength limit; others deform irreversibly, so a given amount of deformation may be considered as the limit for compressive load. Compressive strength is a key value for design of structures.
Compressive strength is often measured on a universal testing machine. Measurements of compressive strength are affected by the specific test method and conditions of measurement. Compressive strengths are usually reported in relationship to a specific technical standard.
Introduction.
When a specimen of material is loaded in such a way that it extends it is said to be in "tension". On the other hand, if the material compresses and shortens it is said to be in "compression".
On an atomic level, the molecules or atoms are forced apart when in tension whereas in compression they are forced together. Since atoms in solids always try to find an equilibrium position, and distance between other atoms, forces arise throughout the entire material which oppose both tension or compression. The phenomena prevailing on an atomic level are therefore similar.
The "strain" is the relative change in length under applied stress; positive strain characterizes an object under tension load which tends to lengthen it, and a compressive stress that shortens an object gives negative strain. Tension tends to pull small sideways deflections back into alignment, while compression tends to amplify such deflection into buckling.
Compressive strength is measured on materials, components, and structures.
By definition, the ultimate compressive strength of a material is that value of uniaxial compressive stress reached when the material fails completely. The compressive strength is usually obtained experimentally by means of a "compressive test". The apparatus used for this experiment is the same as that used in a tensile test. However, rather than applying a uniaxial tensile load, a uniaxial compressive load is applied. As can be imagined, the specimen (usually cylindrical) is shortened as well as spread laterally. A stress–strain curve is plotted by the instrument and would look similar to the following:
The compressive strength of the material would correspond to the stress at the red point shown on the curve. In a compression test, there is a linear region where the material follows Hooke's law. Hence, for this region, "formula_1", where, this time, E refers to the Young's Modulus for compression. In this region, the material deforms elastically and returns to its original length when the stress is removed.
This linear region terminates at what is known as the yield point. Above this point the material behaves plastically and will not return to its original length once the load is removed.
There is a difference between the engineering stress and the true stress. By its basic definition the uniaxial stress is given by:
formula_2
where,
F = Load applied [N],
A = Area [m2]
As stated, the area of the specimen varies on compression. In reality therefore the area is some function of the applied load i.e. A = f(F). Indeed, stress is defined as the force divided by the area at the start of the experiment. This is known as the engineering stress and is defined by,
formula_3
A0=Original specimen area [m2]
Correspondingly, the engineering strain would be defined by:
formula_4
where
l = current specimen length [m] and l0 = original specimen length [m]
The compressive strength would therefore correspond to the point on the engineering stress-strain curve formula_5 defined by
formula_6
formula_7
where
F* = load applied just before crushing and l* = specimen length just before crushing.
Deviation of engineering stress from true stress.
In engineering design practice, professionals mostly rely on the engineering stress. In reality, the "true stress" is different from the engineering stress. Hence calculating the compressive strength of a material from the given equations will not yield an accurate result. This is because the cross sectional area A0 changes and is some function of load A = φ(F).
The difference in values may therefore be summarized as follows:
Comparison of compressive and tensile strengths.
Concrete and ceramics typically have much higher compressive strengths than tensile strengths. Composite materials, such as glass fiber epoxy matrix composite, tend to have higher tensile strengths than compressive strengths. Metals are difficult to test to failure in tension vs compression. In compression metals fail from buckling/crumbling/45deg shear which is much different (though higher stresses) than tension which fails from defects or necking down.
Compressive failure modes.
If the ratio of the length to the effective radius of the material loaded in compression (Slenderness ratio) is too high, it is likely that the material will fail under buckling. Otherwise, if the material is ductile yielding usually occurs which displaying the barreling effect discussed above. A brittle material in compression typically will fail by axial splitting, shear fracture, or ductile failure depending on the level of constraint in the direction perpendicular to the direction of loading. If there is no constraint (also called confining pressure), the brittle material is likely to fail by axial spitting. Moderate confining pressure often results in shear fracture, while high confining pressure often leads to ductile failure, even in brittle materials.
Axial Splitting relieves elastic energy in brittle material by releasing strain energy in the directions perpendicular to the applied compressive stress. As defined by a materials Poisson ratio a material compressed elastically in one direction will strain in the other two directions. During axial splitting a crack may release that tensile strain by forming a new surface parallel to the applied load. The material then proceeds to separate in two or more pieces. Hence the axial splitting occurs most often when there is no confining pressure, i.e. a lesser compressive load on axis perpendicular to the main applied load. The material now split into micro columns will feel different frictional forces either due to inhomogeneity of interfaces on the free end or stress shielding. In the case of stress shielding, inhomogeneity in the materials can lead to different Young modulus. This will in turn cause the stress to be disproportionately distributed, leading to a difference in frictional forces. In either case this will cause the material sections to begin bending and lead to ultimate failure.
Micro-cracks, Leading Cause of Failure in Compression for brittle and quasi brittle material:.
            Micro-cracks are a leading cause of Failure in compression. Sliding along crack tips leads to tensile forces that stretch the along the crack tip. Hence micro cracks will form around any pre-existing crack tips. In all cases it is the overall global compressive stress interacting with local microstructural anomalies to create local areas of tension.  Sources of those pre-existing “crack tips” are listed below:
1.     Porosity is the controlling factor for compressive strength in many materials. These micro-cracks in turn begin to stretch out from the pores, until about they reach approximately the same diameter as the pores, that cause them. (Figure 1 part a)
2.    Stiff inclusions within a material such as a precipitate can cause local areas of tension a certain distance away from the material. (See Fig 1part B below) When inclusions are grouped up (such as in precipitates), this effect can be amplified.
3.    Even without pores or inclusions a material can develop micro-cracks between weak inclined (relative to applied stress) interfaces. These interfaces can slip and create a secondary crack. These secondary cracks continue opening as the slip of the original interfaces acts like a jack, wedging open further the secondary crack. (Fig 1 part C), The slipping of interfaces alone is not solely responsible for secondary crack growth as inhomogeneities in the materials young modulus can lead to an increase effective misfit strain. Cracks that grow this way are known as a wing tip microcracks.
It is important to emphasize that the growth of microcracks is not the growth of the original crack/imperfection. The cracks that are nucleating are doing so perpendicular to original crack and are known as secondary cracks. The figure below emphasizes this point for wingtip cracks.
These secondary cracks can grow to as long as 10-15 times the length of the original cracks in simple (uniaxial) compression. However, if a transverse compressive load is applied. The growth is limited to a few integer multiples of the original crack’s length.
"Shear Bands:".
If the sample size is too big such that the worse defect’s secondary cracks cannot grow large enough to break the sample, other defects within the sample will begin to grow secondary cracks as well. This will occur homogenously over the entire sample. These micro-cracks form an echelon that can form an “intrinsic” fracture behavior, the nucleus of a shear fault instability. Shown right:
Eventually this leads the material deforming non-homogenously. That is the strain caused by the material will no longer vary linearly with the load. Creating localized shear bands on which the material will fail according to deformation theory. “The onset of localized banding does not necessarily constitute final failure of a material element, but it presumably is at least the beginning of the primary failure process under compressive loading.” 
Compressive strength of concrete.
For designers, compressive strength is one of the most important engineering properties of concrete. It is a standard industrial practice that the concrete is classified based on grades. This grade is nothing but the Compressive Strength of the concrete cube or cylinder. Cube or Cylinder samples are usually tested under a compression testing machine to obtain the compressive strength of concrete. The test requirements differ country to country based on the design code. Use of a Compressometer is common. As per Indian codes, compressive strength of concrete is defined as:
"The "compressive strength of concrete" is given in terms of the "characteristic compressive strength" of 150 mm size cubes tested after 28 days (fck). In field, compressive strength tests are also conducted at interim duration i.e. after 7 days to verify the anticipated compressive strength expected after 28 days. The same is done to be forewarned of an event of failure and take necessary precautions. The characteristic strength is defined as the strength of the concrete below which not more than 5% of the test results are expected to fall."
For design purposes, this compressive strength value is restricted by dividing with a factor of safety, whose value depends on the design philosophy used.